Subcategory: 2000 Series Aluminum Alloy; Aluminum Alloy; Metal; Nonferrous Metal
Close Analogs: None
A Zr + Ti limit of 0.20 percent maximum may be used with this alloy designation for extruded and forged products only, but only when the supplier or producer and the purchaser have mutually so agreed. Agreement may be indicated, for example, by reference to a standard, by letter, by order note, or other means which allow the Zr + Ti limit.
Aluminum content reported is calculated as remainder.
Composition information provided by the Aluminum Association and is not for design.
Key Words: Aluminium 2024-O; UNS A92024; ISO AlCu4Mg1; NF A-U4G1 (France); DIN AlCuMg2; AA2024-O, ASME SB211; CSA CG42 (Canada)
|Component|| Wt. %|
|Al||90.7 - 94.7|| |
|Cr||Max 0.1|| |
|Cu||3.8 - 4.9|| |
|Fe||Max 0.5|| |
|Component|| Wt. %|
|Mg||1.2 - 1.8|| |
|Mn||0.3 - 0.9|| |
|Other, each||Max 0.05|| |
|Other, total||Max 0.15|| |
|Si||Max 0.5|| |
|Ti||Max 0.15|| |
|Zn||Max 0.25|| |
General 2024 characteristics and uses (from Alcoa): Good machinability and surface finish capabilities. A high strength material of adequate workability. Has largely superceded 2017 for structural applications. Use of 2024-O not recommended unless subsequently heat treated.
Uses: Aircraft fittings, gears and shafts, bolts, clock parts, computer parts, couplings, fuse parts, hydraulic valve bodies, missile parts, munitions, nuts, pistons, rectifier parts, worm gears, fastening devices, veterinary and orthopedic equipment, structures.
Data points with the AA note have been provided by the Aluminum Association, Inc. and are NOT FOR DESIGN.
|Density||2.78 g/cc||0.1 lb/in³|| AA; Typical|
|Hardness, Brinell||47||47|| AA; Typical; 500 g load; 10 mm ball|
|Ultimate Tensile Strength||186 MPa||27000 psi|| AA; Typical|
|Tensile Yield Strength||75.8 MPa||11000 psi|| AA; Typical|
|Elongation at Break||20 %||20 %|| AA; Typical; 1/16 in. (1.6 mm) Thickness|
|Elongation at Break||22 %||22 %|| AA; Typical; 1/2 in. (12.7 mm) Diameter|
|Modulus of Elasticity||73.1 GPa||10600 ksi|| AA; Typical; Average of tension and compression. Compression modulus is about 2% greater than tensile modulus.|
|Ultimate Bearing Strength||345 MPa||50000 psi|| Edge distance/pin diameter = 2.0|
|Bearing Yield Strength||131 MPa||19000 psi|| Edge distance/pin diameter = 2.0|
|Poisson's Ratio||0.33||0.33|| |
|Fatigue Strength||89.6 MPa||13000 psi|| AA; 500,000,000 cycles completely reversed stress; RR Moore machine/specimen|
|Machinability||30 %||30 %|| 0-100 Scale of Aluminum Alloys|
|Shear Modulus||28 GPa||4060 ksi|| |
|Shear Strength||124 MPa||18000 psi|| AA; Typical|
|Electrical Resistivity||3.49e-006 ohm-cm||3.49e-006 ohm-cm|| AA; Typical at 68°F|
|CTE, linear 68°F||23.2 µm/m-°C||12.9 µin/in-°F|| AA; Typical; Average over 68-212°F range.|
|CTE, linear 250°C||24.7 µm/m-°C||13.7 µin/in-°F|| Average over the range 20-300ºC|
|Heat Capacity||0.875 J/g-°C||0.209 BTU/lb-°F|| |
|Thermal Conductivity||193 W/m-K||1340 BTU-in/hr-ft²-°F|| AA; Typical at 77°F|
|Melting Point||502 - 638 °C||935 - 1180 °F|| AA; Typical range based on typical composition for wrought products 1/4 inch thickness or greater. Eutectic melting is not eliminated by homogenization.|
|Solidus||502 °C||935 °F|| AA; Typical|
|Liquidus||638 °C||1180 °F|| AA; Typical|
|Annealing Temperature||413 °C||775 °F|| |
|Solution Temperature||256 °C||493 °F|| |
References are available for this material.
This information is provided by
MatWeb.com, The Online Materials Database and is reprinted with their permission.
Copyright 1996-2005 by Automation Creations, Inc.
The contents, results, and technical data on this page may not
be reproduced either electronically, photographically or substantively without permission from
Automation Creations, Inc and MatWeb.com. No warranty, neither expressed nor implied, is given
regarding the accuracy of this information. The user assumes all risk and liability in connection with the use of
information from MatWeb.com.